**A STUDY ON THE RELATIONSHIP BETWEEN CORRUGATED BOX **

**PERIMETER AND ITS COMPRESSION STRENGTH FOR 3 PLY BOX OF **

**A, B & E FLUTE PROFILE USING SIMPLIFIED MCKEE FORMULA **

**AND MINI CARTON COMPRESSION TESTER **

**RamnathShenoy, Tanul Maheshwari **

Department of printing and media engineering | Manipal institute of technology, Manipal

**ABSTRACT**

*Box Compression Strength (BCT) can be defined as the measure of the maximum compressive *

*force per unit width that a paper board box can withstand during a compression test till it *

*reaches the buckling stage. It is expressed in kN/m.It is one of the most important property of the *

*paper board package and it helps in determining the staking limitations as well as the overall *

*strength of the package. *

*Usually, a box compression tester is required for conducting the BCS test but within this paper, *

*an effort has been made to find a more accurate BCS (box compression strength) reading by just *

*using the simplified McKee formula. An average difference value was found out between the BCS *

*readings obtained by the tester and the values calculated using the simplified McKee formula for *

*square boxes of increasing perimeter. The fluting used were A, B and E. If this average *

*difference in incorporated in the formula, it may end up increasing the accuracy and hence the *

*functionality of the formula. *

**Keywords- **Compression strength, McKee formula, Simplified McKee, Fluting, Compression
strength tester

**GE-International Journal of Engineering Research **

**Vol. 5, Issue 6, June 2017 Impact Factor- 5.613**

**ISSN(O): 2321-1717, ISSN(P): 2394-420X **

**1. Literature review **
**1.1 Packaging Boards **

According to ISO standards, paperboard is a paper with a basis weight (grammage) above 224

g/m2, but there are exceptions. It can be single- or multi-ply and can be easily cut and formed. It

is lightweight and strong and hence is used in packaging. Sometimes it is referred to as

cardboard, which is a generic, lay term used to refer to any heavy paper pulp–based board [1].

**1.2 Corrugated boards **

Corrugated board is made from the combination of two sheets liners glued to a corrugated inner

medium called the fluting. These layers of paper are assembled in a way which makes the overall

structure much more robust than each layer taken separately.

Corrugated packaging is a versatile, economic, light, robust, recyclable, practical and yet

dynamic form of packaging [1].

**1.2.1 Fluting **

Flutes are the S shaped waves/arches of a corrugated box that makes up the board. This is called

the board‟s corrugation. Flutes are essentially the reinforcement that make up the board. They

run parallel to the depth of the container and give it its rigidity and crushing/stacking strength.

As well as providing stacking strength, flutes also provide insulation that protects products from

sudden temperature changes [3]. Usually, it can be said that larger flutes like „A‟ flute & „B‟

flute profile provide greater strength and cushioning to the containment, while finer flute profiles

[image:2.612.111.505.537.697.2]like „D‟ & „E‟ (mini) provide better ability to be printed and folded.

The types of fluting vary depending upon how many flutes are included per foot, and how thick

the fluting is. By experimenting with flute profiles, designers can vary compression strength,

cushioning strength and thickness. Flutes come in several standard sizes such as A, B, C, E, and

F. Different flute profiles can be combined in one piece of combined board [4].

**1.3Conversion of corrugated boxes **

Separate liner material and fluting material is bought in the form of rolls of packaging boards.

The grammage of this stock depends on the final strength expectation from the converted

corrugated box. The process starts with the conversion of the fluting stock into the fluted board

using a machine called the corrugator. Then, these fluted rolls are cut and stuck to the liner

material to form corrugated board. This board is die cut or slot cut in the desired shape and the

open end is stitched to seal the box.

**1.3.1 Corrugation **

A typical 52 inches corrugator has three fluting rollers- two of these are for fluting the material

and one is pressure roller to press the liner with the glued flute. These fluting rollers are iron

coated and heated. Iron rods, as many as 27 per cylinder, are used to heat these rollers. These

rods can be individually switched on and off to control the temperature of the rollers. The glue

that is used is obviously heat-set.

**1.3.2 Pasting **

Pasting of the single face corrugated board to another corrugated board or liner material is

facilitated by the dual roll pasting machine. The machine has a large glue roller that runs inside

the glue tank. The pressure rollers squeeze a thin layer of this glue and apply it on to the surface

of the material. Viscosity of the glue depends on the paper grammage (G.S.M.). Grammage also

governs the speed at which the machine has to be run. If the gluing does not properly happen in

the pass, it is manually applied in hope of recovering the board.

**1.3.3 Cutting **

**Using manual cutter- **it is done on a manual cutting table which, on one end, is fixed with a
knife arm. The machine is used to manually cut the board material to desired size when the

automatic cutting machine is occupied or dysfunctional. It does not give quality as good as the

**Using rotary cutter- **it has rolling blades that cut lengths and breaths of the board. It also has
creasing rolls that crimps the board to help in folding it.

**Slot cutting machine** is for making slots in the board so that it can be assembled in the shape of
a carton after folding

**1.3.4 Stitching **

Stitching machine is used to create manufacturer‟s joints to seal the cartons from the open end. The stitching wire used can be rust free quality or normal quality based on the customer‟s

requirement. It is a function of the life expected out of the carton.

**1.4 Box compression strength **

Once the conversion of the box is complete, the next biggest task is to check if the quality of the

box is up to the mark. This is generally done by finding out the box compression strength of the

box using a box compression tester or theoretically, by using the simplified McKee formula as

illustrated below [6].

**BCS= 0.6 x ECT x √**𝑡** x √**𝑍

*This is known as the simplified McKee formula. Here, „BCS‟ refers to box compression strength, *
*„ECT‟ refers to edge compression strength, „Z‟ refers to the box perimeter and „t‟ refers to the *

*thickness/caliper of the board used. *

If the box compression performance does not satisfy the standards of its end use, it calls for an

internal audit of the quality standards maintained in the import of raw material, the processes of

conversion, the storage of both the raw and finished undelivered produce and the transport of the

material in and out of the industry. In such cases, other properties of the board that can affect the

box compression strength are examined and adjusted.

**1.4.1 Edgewise Compression Strength (ECT) **

It is defined as the strength displayed by the corrugated board while being subjected to a constant

compressive stress in the direction of the flutes. It is considered to be of significance mainly

because of its high impact on the box compression strength value [1].

According to the McKee formula mentioned above, edge compression strength is concluded,

**1.4.2 Ring Compression Strength (RCT) **

The ring crush test (RCT) is used to determine the ring crush strength or the ring crush resistance

of a paper strip formed into a ring with a standard length and width. The standards and

procedures are followed as per ISO 12192 and TAPPI T 822.

**ECT = 1.28 (RCT of liner material 1 + m RCT of fluting material + RCT of liner material **
**2) **

*Here, „ECT‟ refers to edge compression strength, „RCT‟ refers to the ring compression strength *
*value and „m‟ refers to the take-up factor of the board used. *

Thus, it can be theoretically concluded that ring compression strength is directly related to the

edge compression strength which, in turn is directly related to box compression strength.

**2. Methodology **

**2.1 Conversion of boxes **

The materials used for the experiment are virgin kraft for the liner part of A, B and E flute

boards, semi kraft for the fluting part of the E flute boards and recycled stock for the fluting part

of A and B flute boards.

A total of 18 square boxes were converted as per the procedure mentioned above for this

particular experiment. Only 3 ply board was used for converting these boxes. A development

[image:5.612.110.510.512.663.2]diagram is given below for reference.

Paper rolls are loaded on a 52 inch corrugator machine to accomplish the fluting of the paperboard and blade auto cutter along with dual roll pasting machine is used to prepare

the 3 ply packaging board roll.

To cut these 3 ply sheets into the size of the box, a rotary cutting machine used.

Now this cut and crimped sheet of the box size is taken to the slot cutter to make the slots

which help the flaps of the box fold inwards and so that the stitching flap gets to its

normal size (smaller than the box height).

Rust free quality stitching wire is used on the stitching machine for stitching the open

box.

The box is folded appropriately according to the crimps formed by rotary cutting machine

and the upper and lower flaps are taped using regular brown tape.

**2.2 Conducting the compression test **

18 fair square boxes were used to conduct the box compression test using an industrial

[image:6.612.143.466.375.560.2]grade compression tester. The dimensions used are as follows.

Table 2.1 Perimeter and dimensions of the boxes that are prepared for each fluting.

Box Perimeter

(inches)

Dimensions

(LxBxH)

Type of fluting

28 7x7x7 A,B and E

30 7.5x7.5x7 A,B and E

32 8x8x7 A,B and E

34 8.5x8.5x7 A,B and E

36 9x9x7 A,B and E

38 9.5x9.5x7 A,B and E

**2.3 Calculating BCT using McKee formula **

On the same 3 ply board material which was used for the conversion of boxes, ring compression strength test (RCT) was done. The RCT values obtained were then used to

The following values of material take-up factor (m) was used for calculating the ECT values.

Table 2.2 Fluting styles and their take-up factors

Box compression strength was then, theoretically calculated using the simplified McKee

formula as illustrated in section 1.4.

**3. Research findings and analysis**

Following values of box compression strength were observed when the boxes were tested on an

industrial grade box compression tester which had been calibrated as per the TAPPI standards.

Table 2.3 Box compression tester values for different fluted boxes

LxBxH (inches) Box perimeter

(inches)

Box compression strength (BCT)

in Kgf

A B E

7.5x7.5x7 30 311.3 279.3 117.6

8x8x7 32 314 309.1 119.2

8.5x8.5x7 34 383.9 285.4 119.9

9x9x7 36 382.6 289 119.4

9.5x9.5x7 38 429.2 293.3 120.1

[image:7.612.113.501.363.538.2]Table 2.4 Noted thickness of the boards with the above three flutes

Fluting style Thickness (mm)

A 3.9

B 2.9

E 2.01

[image:8.612.118.493.206.336.2]Following RCT values were obtained in KN/m from the Ring compression tester

Table 2.4 Fluting styles and their ring compression strength values

Fluting style Ring compression test (RCT)

values in KN/m

Liner material Fluting material

A 3.5 2.76

B 3.5 2.76

E 1.31 5.5

Following values of ECT were obtained by using the formula in section 1.4.2

Table 2.4 Fluting styles and their edge compression strength values

Fluting style Edge compression strength

(ECT) in KN/m

A 14.40

B 13.63

E 4.25

Using above observations and simplified McKee formula, following BCS values were calculated

[image:8.612.179.432.421.524.2]Table 2.5 Calculated values for different fluted boxes

LxBxH

(inches)

Box perimeter

(inches)

Box compression strength

(BCT) in Kgf

A B E

7.5x7.5x7 30 470.9 384.2 99.6

8x8x7 32 486.2 396.7 102.9

8.5x8.5x7 34 501.2 409 106.1

9x9x7 36 515.7 420.8 109.1

9.5x9.5x7 38 529.9 432.4 112.1

**3.1 Comparing the tester values with the formula values **

Average of the difference between the BCS values found out by the tester and the values

calculated by the formula came out to be 136.6 for the fluting style A.

311.3 314

383.9 382.6 429.2

470.9 486.2 501.2 515.7

529.9

159.6 172.2

117.3 133.1 _{100.7}

0 100 200 300 400 500 600

30 inches 32 inches 34 inches 36 inches 38 inches

Box

comp

re

ss

ion

s

tren

gth

Box perimeter (inches)

Tester values Formula values

Average of the difference between the BCS values found out by the tester and the values

calculated by the formula came out to be 117.4 for the fluting style B.

Average of the difference between the BCS values found out by the tester and the values

calculated by the formula came out to be 13.28 for the fluting style E.

From the charts, it was clearly indicated that there was a general increase in the BCS value as per

the increase in the value of the box perimeter. This is well reflected by the BCS values obtained

by the tester as they follow a general increasing trend which is similar to that of the BCS values

which were calculated using the simplified McKee formula.

279.3 309.1 285.4 289 293.3

384.2 396.7 409 420.8 432.4

104.9 _{87.6} 123.6 131.8 139.1

0 100 200 300 400 500

30 inches 32 inches 34 inches 36 inches 38 inches

Box comp re ss ion s tren gth

Box perimeter (inches)

### Chart Title

Tester values Formula values

Difference Linear (Difference)

117.6 119.2 119.9 119.4 120.1

99.6 102.9 106.1 109.1 112.1

18 16.3 13.8 _{10.3} _{8}

0 20 40 60 80 100 120 140

30 inches 32 inches 34 inches 36 inches 38 inches

Box comp re ss ion s tren gth

Box perimeter (inches)

### Chart Title

Tester values Formula values

Also, it can be noticed from the above graphs that the line of difference between the tester values

of BCS and the values calculated using the simplified McKee formula is almost horizontal in

nature. This depicts that there resides an almost constant factor that is the difference between the

practical BCS value (found experimentally using a compression tester) and the BCS values

calculated using the formula. This factor is the average of the difference between the two BCS

values and it was found out to be 136.6 for A fluting, 117.4 for B fluting and 13.28 for E fluting.

Slight variations in the values and the reason behind the line not being completely horizontal is

the atmospheric condition (temperature and relative humidity), inconsistency in the similarity of

raw material and error margin of the equipment used which was beyond the computational scope

of this paper.

**4. Conclusion **

The theoretical relation of the box perimeter with the box compression strength for a 3 ply board

box of various fluting profiles (A, B and E) was studied in this paper using the calculated values

from simplified McKee formula and mini box compression strength tester. These readings were

then compared and the average deviation difference value was found out. This can be the first

step towards eliminating the need of a box compression tester to find BCS for the boxes and to

make the simplified McKee formula more accurate. This might help small industries and

startups, for whom purchasing a box compression tester right away is impractical, in maintaining

the quality of the boxes manufactured.

**Reference **

1. RamnathShenoy, Chirag M, Vinod Kumar A, Tanul Maheshwari, *“Determining the *

*Relationship between E Flute Corrugated Board Properties and its Box Compression Strength”,*

International Journal of Research and Innovation in Applied Science (IJRIAS),Volume I, Issue

IX, December 2016.

2. BishwanathChakravarty, *“A Hand Book for Printing and Packaging Technology”*, First

3. Boxmaster, "*Box Basics - Boxmaster*", Internet:

Http://boxmaster.com/products/box-basics/N.p. [Accessed: 15 Mar. 2017].

4. M.C. Kaushal, V.K.Sirohiya and R.K.Rathore, “*Corrugated Board Structure: A Review*”,

International Journal of Application of Engineering and Technology (IJAET), ISSN: 2395-3594,

Vol-2 No.-3.

5. Aaron L. Brody & Kenneth S. Marsh, “*Encyclopedia of Packaging Technology*”, Second

Edition, A Wiley-Interscience Publication, Hoboken, NJ, 1997

6. Roman Popil, “*The BCT of Copy Paper Boxes – Applying McKee‟s Formula*”, Corriexpo,

October 7-9, 2013.

7. Dept. of Printing and Media Engineering, MIT, Quality Testing Lab manual, Manipal, 2013.

8. Niir Board, “*Hand Book on Modern Packaging Industries*”, Asia Pacific Business Press Inc.,